Application of Gold Electrodes for the Study of Nickel Based Homogeneous Catalysts for Hydrogen Oxidation

Article of the journal: JEPT - Journal for Electrochemistry and Plating Technology
Link to the online version of the article: http://www.jept.de/?p=2269
DOI: 10.12850/ISSN2196-0267.JEPT2269

Gold and glassy carbon working electrode materials are compared as suitable substrates for the hydrogen oxidation reaction with Ni(PCy₂Nt-Bu₂)₂(BF₄)₂ used as a catalyst. Voltammetric responses showing electrocatalytic hydrogen oxidation mediated by the homogeneous electrocatalyst Ni(PCy₂Nt-Bu₂)₂(BF₄)₂ are identical at glassy carbon and gold electrodes, which shows that gold electrode can be used for hydrogen oxidation reaction.

Paper: Received: 2013-07-08 / Received in revised form: 2013-08-07 / Accepted: 2013-08-12
Keywords: homogeneous catalysis, hydrogen oxidation, hydrogenase, nickel electrocatalyst, turnover frequency

1. Introduction

The study of homogeneous electrocatalysts for the hydrogen evolution and oxidation reactions contributes to our understanding of hydrogenase enzymes and provides a foundation for the rational development of synthetic catalysts for use in energy technologies. [1-7] Recently, turnover frequencies as high as 50 s⁻¹ for hydrogen oxidation [4] and above 10⁵ s⁻¹ for hydrogen evolution [7] have been observed for functional hydrogenase mimics in acetonitrile solution, with these reversible nernstian catalysts generally operating at proton-coupled mechanism and larger overpotentials than the enzymes themselves. Glassy carbon electrodes are typically used as working electrodes in these studies, as this material is inert for hydrogen oxidation and reduction thus minimizing background currents corresponding to electrode-catalyzed reactions. [1, 3, 4] In this contribution, we will examine the role of the electrode material in studies of homogeneously catalyzed hydrogen oxidation and demonstrate the practicality of gold electrodes as an alternative to glassy carbon.

Gold is active for hydrogen evolution reaction in organic solvents at potentials near that of platinum. [8] However, gold like carbon does not catalyze hydrogen oxidation. [8] The real advantage of gold is that it can be used in electrode configurations that are difficult to achieve with carbon, including but not limited to mesh electrodes for spectroelectrochemical cells, [9, 10] interdigitated array electrodes [11] and scanning electrochemical microscope probe tips [12, 13] where gold electrodes are easy to fabricate. [14-17] Scheme 1 shows the structure of the nickel bis (diphosphine) hydrogen oxidation catalyst Ni(PCy₂Nt-Bu₂)₂²⁺.

Scheme 1: Schematic presentation of Ni(PCy₂Nt-Bu₂)₂²⁺

2. Experimental

Cyclic voltammograms were recorded using an IVIUM compact bipotentiostat (Eindhoven, the Netherlands). A sealed three-electrode cell (ACE Glass, Vineland, NJ) was loaded and assembled in an inert-atmosphere glovebox for all experiments, with a bare silver wire acting as a quasi-reference electrode and a platinum wire or a glassy carbon rod (Alfa Aesar, Ward Hill, MA) as a counter electrode. All potentials for electrochemical experiments were calibrated using the measured E1/2 value for the ferrocene/ferrocenium redox couple (Cp₂Fe+/0, 0 V). Working electrodes (CH instruments, Austin, TX) were gold, glassy carbon (0.5 mm radius) and 1 mm platinum, and were polished with 0.3 μm alumina and thoroughly dried in the flow of nitrogen prior transferring to the glovebox. Benzonitrile was used as a solvent in the catalytic process and for the reaction at platinum electrodes. Hydrogen gas (UHP, Praxair Inc., Danbury, CT) was purified by passage through an oxygen/moisture/hydrocarbon trap (Restek, Bellefonte, PA). Electrochemical grade tetra-n-butylammonium hexafluorophosphate (TBAPF₆), triethylamine (TEA, 99 %) and benzonitrile (99.8 %) were obtained from Sigma-Aldrich (Milwaukee, WI) and used as received.

3. Results and discussion

Figure 1a shows cyclic voltammograms for Ni(PCy₂Nt-Bu₂)₂²⁺ in benzonitrile exhibiting two reversible one-electron waves assigned to the Ni(II/I) and Ni(I/0) redox couples (−0.8 V and −1.45 V vs Cp₂Fe+/0, respectively) [4] at gold electrode. Cyclic voltammograms, with added triethylamine (TEA) and under 1 atm hydrogen, using both glassy carbon and gold electrodes of the same nominal size are shown in Figure 1b. These voltammograms are essentially identical, indicating the suitability of either electrode material in the study of homogeneous catalysis of hydrogen oxidation under these conditions. The increase of current from 0.2 μA to 16 μA because of catalytic process is clearly visible. Turnover frequencies of 48-56 s⁻¹ under 1 atm. hydrogen are calculated and are in the same range as previously reported values. [4] Presence of first order kinetics for nickel catalyst concentration, independence on the base concentration in case of excess of it and according to that an ECcat. (EC’) mechanism was assumed in all calculations: [1]

ic/ip=(n/0.4463)*(RTkobs/Fν)1/2
where kobs is turnover frequency, ic is a catalytic current and ip a peak current for reaction in the absence of catalyst and ν scan rate of the reaction.

Ni(PCy₂Nt-Bu₂)₂²⁺ + H₂ = Ni(PCy₂Nt-BuH₂)₂

Ni(PCy₂Nt-BuH₂)₂   =  Ni(PCy₂Nt-BuH₂)₂ ²⁺ + 2e

Ni(PCy₂Nt-BuH₂)₂²⁺ + TEA = Ni(PCy₂Nt-BuH₂)₂ + (decomposition products)

1b
Fig. 1: Cyclic voltammetry of Ni(PCy₂Nt-Bu₂)₂²⁺ (a) (0.12 mM) and (b) (0.05 mM) in the presence of hydrogen (1 atm) and presence (black and red line) and absence (green line) of 15 mM TEA; insert is an enlarged version of the catalytic current at two different electrodes. Scan rate: 0.05 V s⁻¹; red line corresponds with a carbon electrode and black line with gold electrode; solvent: benzonitrile.

The obtained results are different compared with platinum electrodes, where heterogeneous oxidation waves for hydrogen oxidation appear at more negative potentials compared with the wave for the nickel catalyst, which makes platinum electrode unusable in catalytic investigations (Fig. 2). [8, 18-20] There is a substantial shift of the hydrogen oxidation potential to the negative potentials compared with neutral systems, because of the amines present, though it is still not enough to carry on homogeneous hydrogen oxidation.

Fig. 2: Cyclic voltammograms showing the passivation of a platinum electrode with consecutive scan in the presence of 50 mM triethylamine; scan rate: 0.1 V/s, solvent: benzonitrile.

4. Conclusions

The current work demonstrates that gold electrode is a suitable material for homogeneous hydrogen oxidation in anhydrous solvents, which is very important in case of surface modification studies and kinetics investigations. This can allow achieving application of the nickel catalysts and materials of other nonprecious materials like iron, which can be a viable alternative for commonly applied heterogeneous catalysts such as platinum. Further efforts will be directed to obtain surface modification of gold electrodes to transform currently synthesized homogeneous solution catalysts to the solid catalysts ready to be used in fuel cells. Final goal is to obtain a surface attached catalyst that demonstrates strong catalytic activity in aqueous systems.

Acknowledgement

This work is supported as part of the Center for Molecular Electrocatalysis, an Energy Frontier Research Center funded by the U.S. Department of Energy, Office of Science, Office of Basic Energy Sciences, under FWP 56073. The authors thank Drs. Daniel L. DuBois and R. Morris Bullock for their assistance in preparing the manuscript.

toc
TOC Figure

References

A. D. Wilson, R. H. Newell, M. J. McNevin, J. T. Muckerman, M. Rakowski DuBois and D. L. DuBois, “Hydrogen oxidation and production using nickel-based molecular catalysts with proton relays,” Journal of American Chemical Society, vol. 128, no. 1, pp. 358-366, 2006.

M. O’Hagan, J. W. Shaw, S. Raugei, S. Chen, J. Y. Yang, U. J. Kilgore, D. L. DuBois and R. M. Bullock, “Moving protons with pendant amines: proton mobility in a nickel catalyst for oxidation of hydrogen,” Journal of American Chemical Society, vol. 133, no. 36, pp. 14301-14312, 2011.

A. Le Goff, V. Artero, B. Jousselme, P. D. Tran, N. Guillet, R. Metaya, A. Fihri, S. Palacin and M. Fontecave, “From hydrogenases to nobel metal-free catalytic nanomaterials for H2 production and uptake,” Science, vol. 326, no. 5958, pp. 1384-1387, 2009.

J. Y. Yang, S. Chen, W. G. Dougherty, W. S. Kassel, R. M. Bullock, D. L. DuBois, S. Raugei, R. Rousseau, M. Dupius and M. Rakowski Dubois, “Hydrogen oxidation catalysis by a nickel diphosphine complex with pendant tert-butyl amines,” Chemical Communications, vol. 46, no 45, pp. 8618-8620, 2010.

M. T. M. Koper and E. Bowman, “Electrochemical hydrogen production: bridging homogeneous and heterogeneous catalysis,” Angewandte Chemie. International Edition, vol. 49, no. 22, 3723-3725, 2010.

U. J. Kilgore, J. A. S. Roberts, D. H. Pool, A. M. Appel, M. P. Stewart, M. Rakowski Dubois, W. G. Dougherty, W. S. Kassel, R. M. Bullock and D. L. DuBois, “[Ni(PPh₂NC6H4X₂)₂]²⁺ complexes as electrocatalysts for H₂ production: effect of substituents, acids, and water on catalytic routes,” Journal of American Chemical Society, vol. 133, no. 15, pp. 5861-5871, 2011.

M. L. Helm, M. P. Stewart, R. M. Bullock, M. Rakowski DuBois and D. L. DuBois, “A synthetic nickel electrocatalyst with a turnover frequency above 100000 s⁻¹ for H₂ production,” Science, vol. 333, no. 6044, pp. 863-866, 2011.

W. C. Barrette and D. T. Sawyer, “Determination of dissolved hydrogen and effects of media and electrode materials on the electrochemical oxidation of molecular hydrogen,” Analytical Chemistry, vol. 56, no. 3, pp. 653-657, 1984.

H. O. Finklea, R. K. Boggess, J. W. Trogdona and F. A. Schultz, “Thin-layer spectroelectrochemistry cell with demountable gold or mercury-gold minigrid electrodes,” Analytical Chemistry, vol. 55, no. 7, 1177-1179, 1983.

S. H. Kim, J. W. Lee and I. H. Yeo, “Spectroelectrochemical and electrochemical behavior of epinephrine at a gold electrode,” Electrochimica Acta, vol. 45, no. 18, 2889-2895 (2000).

B. J. Seddon, H. H. Girault and M. J. Eddowes, “Interdigitated microband electrodes: chronoamperometry and steady state currents,” Journal of Electroanalytical Chemistry, vol. 266, no. 2, 227-238, 1989.

B. Liu and A. J. Bard, “Scanning electrochemical microscopy. Study of the kinetics of oxygen reduction on platinum with potential programming of the tip,” Journal of Physical Chemistry B, vol. 106, no.49, 12801-12806, 2002.

A. Minguzzi, M. A. Alpuche-Aviles, J. Rodriguez-Lopez, S. Rondinini and A. J. Bard, “Screening of oxygen evolution electrocatalysts by scanning electrochemical microscopy using a shielded tip approach.” Analytical Chemistry, vol. 80, no. 11, pp. 4055-4064, 2008.

J. Velmurugan, P. Sun and M. V. Mirkin, “Scanning electrochemical microscopy with gold nanotips: the effect of electrode material on electron transfer rates,” Journal of Physical Chemistry C, vol. 113, no. 1, pp. 459-464, 2009.

B. Zhang, J. Galusha, P. G. Shiozawa, G. Wang, A. J. Bergen, R. M. Jones, R. M. White, E. N. Ervin, C. C. Cauley and H. C. White, “Bench-top method for fabricating glass-sealed nanodisk electrodes, and glass nanopore membranes of controlled size,” Analytical Chemistry, vol. 79, no. 13, pp. 4778-4787, 2007.

P. Sun and M. V. Mirkin, “Kinetics of electron-transfer reactions at nanoelectrodes,” Analytical Chemistry, vol. 78, no. 18, pp. 6526-6534, 2006.

S. P. Forry and R. M. Wightman, “Electrogenerated chemiluminescence detection in reversed-phase liquid chromatography,” Analytical Chemistry, vol. 74, no. 3, pp. 528-532, 2002.

D. S. Silvester, K. R. Ward, L. Aldous, C. Hardacre and R. G. Compton, “The electrochemical oxidation of hydrogen at activated platinum electrodes in room temperature ionic liquids as solvents,” Journal of Electroanalytical Chemistry, vol. 618, no. 1-2, pp. 53-60, 2008.

B. E. Conway and D. M. Novak, “Thermodynamics of ethanol at low concentrations in mixtures of cycloxehane and 1,4-dimethylbenzene,” Journal of Physical Chemistry, vol. 81, no. 15, 1459-1468, 1977.

S. Trasatti, “Work function, electronegativity and electrochemical behavior of metals. Electrolytic hydrogen evolution in acid solutions,” Journal of Electroanalytical Chemistry, vol. 39, no. 1, pp. 163-184, 1972.

Authors:

Alexander B. Nepomnyashchii

Alexander Nepomnyashchii obtained the specialist degree in Chemistry and English in 2001 and Candidate of Science in Physical Chemistry in 2005 from Herzen State Pedagogical University of Russia (Saint Petersburg, Russia). During this time he worked under the supervision of Dr. Vyacheslav Nickolaevich Pak. He obtained his Master of Science degree in 2004 from University of Northern Iowa, where he worked under the supervision of Dr. Shoshanna R. Coon. He completed his Ph. D. degree in Analytical Chemistry at the University of Texas, Austin in 2011 under the direction of Dr. Allen J. Bard. He is currently a post-doctoral associate of Dr. Bruce A. Parkinson at University of Wyoming.

Address: Department of Chemistry and School of Energy Resources, University of Wyoming, Laramie, Wyoming 82071, United States, Email: anepomny@uwyo.edu

Fei Liu

Fei Liu obtained her B. S. in 2005 and M. S. in 2008 degrees from Xian Jiaotong University. She is currently a fourth year Ph. D. student at the University of Wyoming.

Address: Department of Chemistry and School of Energy Resources, University of Wyoming, Laramie, Wyoming 82071, United States

John A. S. Roberts

John A. S. Roberts obtained his B. S. degree in Mathematics from University of Wisconsin (Madison) in 2001 and Ph. D. in Chemistry from Northwestern University in 2006. He worked during his graduate studies under the supervision of Dr. Tobin J. Marks. He was a post-doctoral associate at the Pacific Northwest National Laboratory (PNNL) from 2006 to 2009. He is currently a staff scientist at PNNL.

Address: Chemical and Physical Sciences Division, Pacific Northwest National Laboratory, P. O. Box 999, K2-57, Richland, Washington 99352, United States

Prof. B. A. Parkinson

Prof. B. A. Parkinson obtained his B.S. degree at Iowa State University in 1972 and his Ph. D. from California Institute of Technology in 1977 working in Dr. Fred C. Anson laboratory. He completed his postdoctoral investigations at Bell laboratories, where he worked under the supervision of Adam Heller. He then worked as a staff scientist at the Ames laboratory (1979-1981), a senior scientist at the Solar Energy Research Institute in Golden (1981-1985) and Central Research and Development Department of DuPont Company (1985-1991). He became a professor of Chemistry at Colorado State University in 1991 and he moved to the University of Wyoming in 2008. He is currently J. E. Warren Professor of Energy and Environment and School of Energy Resources (SER) professor of Chemistry.

Address: Department of Chemistry and School of Energy Resources, University of Wyoming, Laramie, Wyoming 82071, United States, Email: bparkin1@uwyo.edu

Contact

EUGEN G. LEUZE VERLAG KG

Ralf Schattmaier

Karlstraße 4

88348 Bad Saulgau

Germany

Website: www.jept.de

Email: ralf.schattmaier@leuze-verlag.de

Phone: +49 0 7581 4801-12

Fax: +49 0 7581 4801-10